Rational Assembly of Co/Cd-MOFs Featuring Topological Variation
Wang, Hao; Yi, Fei-Yan; Dang, Song; Tian, Wan-Guo; Sun, Zhong-Ming; Crystal Growth & Design 14 (2014) 147–; doi:10.1021/cg4013334

data_4509984
_publ_section_title
;
 Rational Assembly of Co/Cd-MOFs Featuring Topological Variation
;
_journal_issue                   1
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              147
_journal_paper_doi               10.1021/cg4013334
_journal_volume                  14
_journal_year                    2014
_chemical_formula_sum            'C31 H26 Cd N6 O11'
_chemical_formula_weight         770.98
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 91.8990(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.2450(4)
_cell_length_b                   16.1456(8)
_cell_length_c                   26.6414(13)
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      26.10
_cell_measurement_theta_min      1.47
_cell_volume                     3114.7(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0280
_diffrn_reflns_av_sigmaI/netI    0.0328
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            16953
_diffrn_reflns_theta_full        26.10
_diffrn_reflns_theta_max         26.10
_diffrn_reflns_theta_min         1.47
_exptl_absorpt_coefficient_mu    0.774
_exptl_absorpt_correction_T_max  0.7453
_exptl_absorpt_correction_T_min  0.6559
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Sheldrick, G. M. (2008). SADABS'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.644
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1560
_exptl_crystal_size_max          0.42
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_refine_diff_density_max         2.733
_refine_diff_density_min         -0.554
_refine_diff_density_rms         0.103
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.008
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     442
_refine_ls_number_reflns         6135
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.008
_refine_ls_R_factor_all          0.0491
_refine_ls_R_factor_gt           0.0414
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0635P)^2^+6.7108P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1099
_refine_ls_wR_factor_ref         0.1155
_reflns_number_gt                5268
_reflns_number_total             6135
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg4013334_si_002.cif
_cod_data_source_block           2
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               4509984